# Synthesis of the Titanium Oxides Using a New Microwave Discharge Method

Marian Mogildea, George Mogildea, Sorin I Zgura, Gabriel Chiritoi, Cristian Ionescu, Valentin Craciun, Petronela Prepelita, Natalia Mihailescu, Alexandru Paraschiv, Bogdan Stefan Vasile, et al.

► To cite this version:

Marian Mogildea, George Mogildea, Sorin I Zgura, Gabriel Chiritoi, Cristian Ionescu, et al. Synthesis of the Titanium Oxides Using a New Microwave Discharge Method. International Journal of Molecular Sciences, 2025, 26, 10.3390/ijms26052173. [DOI] [Full Text]
Article

# Synthesis of the Titanium Oxides Using a New Microwave Discharge Method

Marian Mogildea<fnref n="1" />, George Mogildea <fnref n="1" />,* ID, Sorin I. Zgura ¹ID, Gabriel Chiritoi <fnref n="1" />, Cristian Ionescu <fnref n="1" />, Valentin Craciun <fnref n="2" />,<fnref n="3" /> ID, Petronela Prepelita <fnref n="2" />, Natalia Mihailescu <fnref n="2" />, Alexandru Paraschiv <fnref n="4" /> ID, Bogdan Stefan Vasile <fnref n="5" />,<fnref n="6" /> ID and Catalin Daniel Constantinescu <fnref n="7" /> ID

<figure><img src="image_1.png" /></figure>

check for
updates

Academic Editor: Zoltán Dudás

Received: 28 January 2025

Revised: 21 February 2025

Accepted: 24 February 2025

Published: 28 February 2025

**Citation:** Mogildea, M.; Mogildea, G.; Zgura, S.I.; Chiritoi, G.; Ionescu, C.; Craciun, V.; Prepelita, P.; Mihailescu, N.; Paraschiv, A.; Vasile, B.S.; et al. Synthesis of the Titanium Oxides Using a New Microwave Discharge Method. *Int. J. Mol. Sci.* **2025**, *26*, 2173. https://doi.org/10.3390/ijms26052173

**Copyright:** © 2025 by the authors.
Licensee MDPI, Basel, Switzerland.
This article is an open access article
distributed under the terms and
conditions of the Creative Commons
Attribution (CC BY) license
(https://creativecommons.org/
licenses/by/4.0/).

**Abstract:** This research highlights the different behaviors of titanium (Ti) wires under the action of 500 W and 800 W microwave power levels. Following the interaction between microwaves and a titanium wire placed in the node of the (TM₀₁₁—transverse magnetic mode) waveguide in air at atmospheric pressure, plasma was generated. Using optical emission spectroscopy technique it was observed that during plasma generation at 500 W and 800 W microwaves powers, metallic ions, and gas ions were created, and the plasmas fulfilled the local thermodynamic equilibrium (LTE) conditions. The XRD analysis showed that on the surface of the Ti wire exposed to 500 W microwave power a mixture of titanium dioxide (TiO₂) and titanium oxide (TiO) grew, while the Ti wire exposed to 800 W microwave power was completely vaporized and a mixture of TiO₂ and TiO nanoparticles was synthesized. The SEM analysis showed that the dimensions of the titanium oxide (TiOₓ) nanoparticles generated by both microwave discharges ranged from 5 nm to 200 nm. The results of EDS analysis showed that the power of microwaves plays an important role in quantitative conversion from Ti wire into a TiOₓ mixture. The TEM analysis indicates that most of the nanoparticles are either amorphous or nanocrystalline. Using this simple and inexpensive technique one can grow a TiOₓ layer on the surface of titanium electrodes or can synthetize nanocrystalline TiOₓ particles.

**Keywords:** microwaves; plasma; nanoparticles

## 1. Introduction

Titanium oxides (TiOₓ) are naturally occurring compounds used for many years in various branches of industry [1]. TiOₓ is a non-toxic substance that possesses antibacterial properties [2,3] and has excellent biocompatibility with organic cells [3,4]. TiOₓ in powder form [5] is used in commercial applications as pigments, in the food industry as a coloring additive, and in the pharmaceutical domain as a protector of active ingredients against light

<footnote n="1">¹ Institute of Space Science—Subsidiary of the National Institute for Laser, Plasma and Radiation Physics, 077125 Magurele, Romania; marian_mogildea@spacescience.ro (M.M.); szgura@spacescience.ro (S.I.Z.); gabriel.chiritoi@spacescience.ro (G.C.); idcristi@gmail.com (C.I.)</footnote>

<footnote n="2">² National Institute for Laser, Plasma and Radiation Physics, 409 Atomistilor st., 077125 Magurele, Romania; valentin.craciun@inflpr.ro (V.C.); petronela.garoi01@gmail.com (P.P.); natalia.serban@inflpr.ro (N.M.)</footnote>

<footnote n="3">³ Extreme Light Infrastructure for Nuclear Physics, 077125 Magurele, Romania</footnote>

<footnote n="4">⁴ Romanian Research & Development Institute for Gas Turbines, 061126 Bucharest, Romania; alexandru.paraschiv@comoti.ro</footnote>

<footnote n="5">5 National Research Center for Micro and Nanomaterials, Bucharest National Polytechnic University of Science and Technology, 060042 Bucharest, Romania; vasile_bogdan_stefan@yahoo.com</footnote>

<footnote n="6">⁶ Research Center for Advanced Materials, Products and Processes, Bucharest National Polytechnic University of Science and Technology, 060042 Bucharest, Romania</footnote>

<footnote n="7">7 CNRS, LP3 UMR 7341, Aix-Marseille University, 13009 Marseille, France; catalin constantinescu@cnrs.fr</footnote>

<footnote>* Correspondence: george_mogildea@spacescience.ro</footnote>
radiation [6]. The deposition of thin films or coatings on the surfaces of other materials with TiO₂ allows for the development of new materials with interesting physical and chemical properties. Until now, TiO₂ and TiO thin films were successfully synthesized by chemical and physical techniques such as chemical bath deposition (CBD) [7], chemical vapor deposition (CVD) [8], molecular beam epitaxy (MBE) [9], RF magnetron sputtering, electrodeposition [10], and pulsed laser deposition (PLD) [11].

Current technologies based on plasma generation have low efficiency and incomplete conversion of the titanium to TiO₂ [12,13]. Moreover, these systems contain mechanical and electronic modules that are very expensive, have large dimensions, and cannot be easily installed in another workspace. The chemical techniques are less expensive, but they have limitations in terms of mass manufacturing, special condition requirements, as well as the use of toxic or poisonous chemicals that endanger human health and the environment [14]. In addition, after the manufacture of the nanoparticles, it is necessary to implement procedures for washing and drying the nanoparticles. These procedures require time and money spent, which leads to a higher cost of producing nanoparticles. Considering that the demand for TiOₓ nanoparticles and new materials based on TiOₓ is increasing, our study investigated the growth of TiOₓ directly on the surface of titanium wires and the synthesis of TiOₓ nanoparticles using a new microwave plasma method. The interaction processes of microwaves with dielectric materials and metals are very well documented. It is known that microwaves are reflected by bulk metals and are absorbed by dielectric materials (gaseous, liquids, plastic, and ceramic materials). Following the absorption process of microwaves by dielectric materials, they are heated up and melted, and for very large powers a plasma is created [15]. Recently, studies were performed on the heating of metal powders under the action of microwaves. The results showed that the physical processes occurring during the interaction between microwaves and metal particles are of an electrical nature. When the metallic particles are mixed with liquid substances and are exposed to the microwave field, the liquids heat up due to the occurrence of electrical discharges between the particles [16]. Or, when the metal powder is in a gaseous atmosphere and is exposed to microwaves, it heats up through the occurrence of Eddy currents [17]. Currently, we have a good understanding of the physical processes occurring during the interaction between small metallic objects (feature size < 1 mm) and microwaves. Studies have been carried out on the interaction of microwaves and electrons in vacuum and gaseous atmospheres. Research carried out in a vacuum has shown that when a metal electrode is exposed to a microwave field, electrons are generated through the field emission process [18]. Other experiments showed that when the electrodes of a photomultiplier detector interact with microwaves an electrical signal at the output of the photomultiplier is generated [19]. Popescu S. et al. [20] showed that in atmospheric air conditions, a plasma can be created between two titanium pieces brought into contact when these were irradiated with microwaves. In 2018, Yukun Feng et al. [21] introduced a quartz glass cylinder containing paper clips and gaseous acetone into a microwave oven. Following the interaction between the microwaves and the metallic paper clips, electric sparks were generated, and the acetone was decomposed. Other research performed in air or CO₂ atmospheres has shown that when a metal electrode is exposed to a microwave field at a certain power level, plasma is generated and the metallic electrode is vaporized [22]. From these studies, it was observed that during the interaction of microwaves with metallic wires, two physical processes are involved: field emission and the thermionic emission process [23]. The field emission is responsible for plasma initiation and the thermionic process is responsible for the ion generation and vaporization of the metallic wire.
Therefore, the microwave plasma method described in this paper uses the same physical process to generate a plasma, which is oxidizing an electrically insulated titanium wire at low power and synthesizing titanium oxide nanoparticles at high power levels.

Considering that numerous studies have been carried out recently on the interaction of metal powders/wires or small metal objects with microwaves of a certain power, this work highlights different behaviors of Ti wires under the action of low and high microwave power levels. Moreover, using this inexpensive method one can obtain a high-efficiency conversion of the titanium in crystalline $TO_x$ powder nanoparticles and grow the $TO_x$ layers on the surface of the Ti electrodes in atmospheric air.

## 2. Results

To determine the plasma parameters, the plasma was investigated using the optical emission spectroscopy method. An Ocean Optics USB 2000 ++ spectrometer linked to an optical fiber (Ocean Optics Inc., Orlando, FL, USA) was used to record the optical spectrum of the plasma [24]. The integration time of the USB 2000 ++ software was set at 10 ms. Before starting the measurements, and the spectrometer was calibrated using a broadband light source (Ocean Optics DH-mini UV-Vis-NIR Deuterium—Halogen Light Source). After data acquisition, the emission spectrum of the plasma was compared with the NIST database [25]. The optical emission spectra of the plasma generated at 500 W and 800 W microwave power are displayed in Figures 1 and 2, respectively. As one can observe, the emission lines of excited atoms and ions from the atmosphere ($O_2$ and $N_2$) and wire (Ti) are present in the acquired spectra.

<figure><img src="image_2.png" /><figcaption>**Figure 1.** The optical emission spectrum of the plasma generated at 500 W microwave power.</figcaption></figure>

To evaluate if the plasma is at local thermodynamic equilibrium (LTE), the electronic temperature of the plasma was determined using the Boltzmann method [26].

The plots for the plasmas generated using 500 W and 800 W microwave power are displayed in Figure 3 and Figure 4, respectively.

During plasma generation different behaviors of titanium wires depending on the microwave power were observed. For the Ti wire exposed to 500 W microwave power, a thick layer of Ti oxide was formed on the surface of the wire (see Figure 5), while for the Ti wire exposed to 800 W microwave power, this was vaporized (Figure 6) and Ti oxide was deposited on the walls of the waveguide and a silicon substrate placed inside the waveguide to collect the generated nanoparticles for further analysis.
<figure><img src="image_3.png" /><figcaption>**Figure 2.** The optical emission spectrum of the plasma generated at 800 W microwave power.</figcaption></figure>

<figure><img src="image_4.png" /><figcaption>**Figure 3.** The Boltzmann plot of the plasma generated at 500 W microwave power.</figcaption></figure>

<figure><img src="image_5.png" /><figcaption>**Figure 4.** The Boltzmann plot of the plasma generated at 800 W microwave power.</figcaption></figure>
<figure><img src="image_6.png" /><figcaption>**Figure 5.** (a) Optical microscope images of the Ti wire after exposure to 500 W microwave power (magnification 300×): 1—the point where the needle for the adhesion testing instrument was fixed on TiO₂; 2—the point where Ti oxide was exfoliated from the titanium wire. (b) Titanium wire after exfoliation of Ti oxide (magnification 300×), 1—the point where the instrument needle was fixed for the adhesion testing.</figcaption></figure>

<figure><img src="image_7.png" /><figcaption>**Figure 6.** Images of the Ti wire before (a) and after exposure (b) to the microwave field.</figcaption></figure>

In Figure 5a, an optical microscope image of the Ti wire after exposure at 500 W microwave power shows that the wire was oxidized along a length of 3 mm starting from the tip.

In Figure 6a,b images of the Ti wire before and after exposure to 800 W microwave power are displayed. Before starting the plasma generation process, the tip of the Ti wire was 5 mm long. After 10 s when the plasma generation process was stopped, the tip of the titanium wire was completely vaporized (see yellow zone in Figure 6b).

To determine the morphology and oxidation state of the Ti oxide synthesized during microwave discharge, the tip of the Ti wire exposed to 500 W microwave power and particles deposited on the silicon substrate obtained at 800 W microwave power were analyzed using EDS, SEM, TEM, and XRD. A high-resolution scanning electron microscope (HRSEM) was used for topographic analysis of samples as well as to observe the structural quality and surface morphology of samples. More precisely, the Apreo microscope from FEI (Thermo Fisher Scientific, Waltham, MA, USA) allows a 0.9 nm resolution. By using HRSEM, we studied the surface of the samples at different magnifications, in a high vacuum, by scanning them with a beam of accelerated electrons at very high energies (≈20 keV) from a 14 cm to 10 cm working distance and an electrical current from 0.1 nA to 13 pA. Prior to imaging analysis, a thin layer of gold was sputtered onto the sample surfaces to avoid electrostatic charging during measurements. For compositional analyses, the system
was equipped with an X-ray source and an EDX unit with elementary energy dispersion spectroscopy (EDS), a fixed silicon detector, and an integrated Peltier element as a cooling system. For EDX, it was operated at 25 kV acceleration voltage, 3.2 nA electrical current, and the dead time was 34 s. EDX measurements were applied at 2.000× magnification. The quantitative elemental analyses were done using TEAM™ v.4.5 software. Figure 7 displays the EDS spectrum acquired from the surface of the Ti wire after exposure to 500 W microwave power and Table 1 displays the chemical composition of the TiOx.

<figure><img src="image_8.png" /><figcaption>**Figure 7.** EDS spectrum of the TiOx from the Ti wire surface.</figcaption></figure>

<table><caption>**Table 1.** The chemical composition of the TiOx from the Ti wire surface.</caption><thead><tr><td>Element</td><td>Weight %</td><td>Atomic %</td></tr></thead><tbody><tr><td>O K</td><td>36.95</td><td>63.7</td></tr><tr><td>Ti K</td><td>63.05</td><td>36.3</td></tr></tbody></table>

In Figure 8 the SEM image (60,000× magnification) of the tip of the Ti wire after exposure to 500 W microwave power is displayed. The sizes of nanoparticles from the surface of the Ti wire ranged between 5 nm and 200 nm.

Figure 9 displays the XRD patterns acquired from the surface of the Ti wire exposed to 500 W microwave power irradiation and their analysis using the Malvern Panalytical software package (https://www.malvernpanalytical.com/en/products/category/x-ray-diffractometers). The observed diffraction peaks correspond to TiO₂ anatase and several TiO phases. No metallic Ti peaks were observed, an indication that the formed oxide layer was rather thick.

The EDS, SEM and XRD analyses performed on the nanoparticles collected on the silicon substrate during vaporization of the Ti wire at 800 W microwave power showed that they have dimensions between 5 nm and 200 nm and consist of a mixture of TiO₂ and TiO. Figure 10 displays the EDS spectrum acquired from the nanoparticles deposited on the silicon substrate at 800 W microwave power and Table 2 displays the chemical composition of the TiOx.
<figure><img src="image_9.png" /><figcaption>**Figure 8.** SEM image of the titanium wire irradiated with 500 W microwaves.</figcaption></figure>

<figure><img src="image_10.png" /><figcaption>**Figure 9.** XRD analysis of the titanium oxide layer synthesized on the surface of the titanium wire by 500 W irradiation.</figcaption></figure>

<figure><img src="image_11.png" /><figcaption>**Figure 10.** EDS spectrum of the TiOₓ nanoparticles from the silicon substrate.</figcaption></figure>
<table><caption>**Table 2.** The chemical composition of the TiOₓ nanoparticles synthesized at 800 W microwave power.</caption><thead><tr><td>Element</td><td>Weight %</td><td>Atomic %</td></tr></thead><tbody><tr><td>O K</td><td>46.14</td><td>71.95</td></tr><tr><td>Ti K</td><td>53.86</td><td>28.05</td></tr></tbody></table>

Figure 11 displays an SEM image of the nanoparticles deposited on the silicon substrate from Ti wire irradiated at 800 W microwave power.

<figure><img src="image_12.png" /><figcaption>**Figure 11.** SEM image of the nanoparticles deposited on the silicon substrate.</figcaption></figure>

The XRD analysis (see Figure 12) of the nanoparticles collected on the Si substrate indicates that their composition is a mixture of TiO and TiO₂. However, the diffraction peaks are smaller and wider than those obtained from the metallic wire irradiated at 500 W. Some TiO₂-SiO₂ mixture, formed because the plasma was very hot and interacted with the Si substrate, was also identified in the collected material.

<figure><img src="image_13.png" /><figcaption>**Figure 12.** XRD analysis of the Ti oxide nanoparticles deposited on the Si substrate.</figcaption></figure>

Figure 13a,b show images of the Ti oxide nanoparticles deposited on the Si substrate using the transmission electron microscopy (TEM) technique. Figure 13c shows the selected area electron diffraction obtained from these particles, which indicates that most of the nanoparticles are either amorphous or nanocrystalline. In the high-resolution TEM image of the nanoparticles displayed in Figure 13b, some regions where interference fringes are visible can be observed, indicative of small crystalline regions.
<figure><img src="image_14.png" /><figcaption>**Figure 13.** (a) Bright-field TEM image of the Ti oxides nanoparticles, (b) high-resolution TEM image of the nanoparticles, and (c) selected area electron diffraction pattern acquired from the nanoparticles.</figcaption></figure>

After turning off the plasma generation, it was noticed that the titanium oxide nanoparticles deposited on the Si substrate at 800 W microwave power were very easy to brush off, while the oxide layer grown on the tip of the Ti wire exposed to 500 W microwave power had strong adhesion. To determine the adhesion of the Ti oxide formed on the tip of the Ti wire when this was exposed to 500 W microwave power, a Revetest Anton Paar instrument was used. The adhesion analyses of a film deposited on a substrate were estimated from the controlled scratching with a diamond-tipped needle (200 µm diameter of the needle tip) on the surface of the object. The test parameters were set at 2 mm/min advance with the depth force progressively increased between 0 N and 100 N.

In Figure 5b one can see the scratch performed by the needle of the instrument on the surface of the microwaves exposed Ti wire. During the adhesion testing, it was observed that when the needle of the instrument penetrated 0.2 mm into the sample, it exfoliated the oxide film from the wire. Figure 14 displays the graph of TiOₓ adhesion versus pressing force on the surface of the titanium wire.

<figure><img src="image_15.png" /><figcaption>**Figure 14.** Adhesion analysis of TiOₓ layer on the Ti wire.</figcaption></figure>

The analysis displayed in Figure 14 shows that the TiOₓ layer was exfoliated at ~50 N pressing force, (at ~1 mm at the interface between metal and TiOₓ). After removing the oxide layer, it was noticed that it was very hard and brittle.

**3. Discussion**

Microwaves are defined in the electromagnetic spectrum as non-ionizing radiation because the photons do not have enough energy to ionize the substance. However, it has
been observed that when microwaves interact directly with wires or small metallic objects in a gaseous atmosphere, ions are generated. The triggering factor in the plasma initiation process is the field emission phenomenon. To initiate a plasma in air at atmospheric pressure when microwaves interact with a metal wire, a main condition must be met: the power of the microwaves must be high enough to induce in wire a high electrical field. The magnitude of this electric field depends on several parameters: the length and diameter of the metal wire, its electrical conductivity, and the power of the microwaves. Therefore, the electrical voltage induced by microwaves in a metal wire can be summarized by two parameters: the ohmic resistance of the metal wire calculated for alternating current ($R_{AC}$) and the power of the microwaves in the focal point of the waveguide. Considering that the $R_{AC}$ of the titanium wire (5 cm length) calculated for the frequency of 2.45 GHz at 20 °C is 437 Ohm, the electrical voltage induced by microwaves in the titanium wire is 46.7 kV for 500 W microwave power and 59.2 kV for 800 W microwave power [27]. At a value of 59.2 kV, the breakdown of the air is initiated, and a plasma is formed. For lower values, the plasma is not initiated. Therefore, to initiate the plasma in air at atmospheric pressure, the power of the microwaves was increased to 800 W. After the plasma initiation process is started, the power of the microwaves can be decreased. From the last figure in Section 4 one can note that the plasma column generated at 500 W microwave power is much smaller than the plasma column generated at 800 W. In Figures 1 and 2 one can observe that during microwave discharges obtained at 500 W and 800 W RF, both plasmas emit spectral lines corresponding to ions from gas and metal wire. To determine the plasma sustaining conditions under 800 W microwave power, the local thermodynamic equilibrium (LTE) conditions for both plasmas (500 W vs. 800 W microwave power) were evaluated. In Figures 3 and 4 it can be observed that both plasmas have fulfilled the conditions of LTE. The plasma-initiating process is caused by the collision between the electrons emitted by the wire and the molecules of the air, in this process, a large amount of heat is generated. The process of electron-atom collision triggers the thermionic emission. After the thermionic emission occurs, the microwave power can be reduced. Therefore, the plasma sustaining process at microwave powers below 800 W is due to the initiating of the thermionic emission. If the microwave power is reduced below 500 W microwave power, the plasma is not initiated. During microwave discharges (500 W and 800 W microwave powers) a mixture of TiO and $TiO_2$ nanoparticles was generated. From the analysis of Figure 5a,b, we noticed that, although there is a large amount of the $TiO_2$ and TiO mixture at the tip of the titanium wire after exfoliation of the titanium oxide, the titanium wire has almost the same diameter. Therefore, during plasma generation the surface of the Ti wire was oxidized uniformly. Additionally, one can notice that at 500 W microwave power, the Ti wire did not vaporize in the focal point of the waveguide and Ti oxide was generated on the surface of the Ti wire.

At 800 W microwave power, the Ti wire was completely vaporized in the focal point region of the waveguide and a large number of nanoparticles of the Ti oxide were deposited on the waveguide walls. Given that in a microwave discharge a lot of heat is produced, the hot air flow induced by the plasma generated at 800 W microwave power carried away the oxide particles from the Ti wire towards the walls of the waveguide. At 500 W of microwave power, the vaporization of the Ti wire is significantly slower, and not enough heat was generated to form an airflow strong enough to carry the synthetized nanoparticles. In Figure 5a (1000× magnification) one can notice that the surface of the titanium oxide layer has an irregular shape with small bumps, which indicates that the Ti oxide has reached the boiling point. Due to the very high temperature generated by the plasma, the Ti oxide melted and then the liquid accumulated at the tip of the titanium wire. If one compares the EDS analysis performed on the two samples (silicon substrate
deposited with TiOₓ and Ti wire covered with TiOₓ layer), it is observed that microwave power plays an important role in quantitative conversion from Ti wire to TiOₓ. By using this microwave plasma generation method, Ti oxide powders or Ti oxide coatings can be obtained on the surface of Ti wires depending on the microwave power. To oxidize a metal wire over a longer length than that observed during these experiments, once the microwave discharge has been initiated, the wire should be continuously advanced through the focal point of the waveguide.

The main advantages of the new microwave plasma method are high production efficiency, a complete conversion of the Ti wire into TiOₓ nanoparticles, and synthesis of crystalline TOₓ nanoparticles even if the atmospheric air contains water vapor [28,29] or other impurities. Moreover, the microwave device is a portable system (it weighs around 12 kg, the dimensions are 0.5 m length, 0.5 m width, and 0.2 m height), it can be installed anywhere, and it does not require special rules/authorizations for use as in the case of using lasers or storage of compressed gas cylinders. This very simple and inexpensive microwave device can be applied in the commercial field, in dental implant processing, or in the field of green energy. Due to the UV radiation reflection properties of Ti oxides [30], these powders can be used in the commercial domain as raw material in sunscreen manufacturing or other applications. Using this microwave plasma method for dental implant coating can improve their biocompatible and osseointegration properties. Considering that TiO₂ is antimicrobial and that rough implant surfaces can increase bone-to-implant contact [31], the lifespan of an implant can be extended by depositing a layer of TiO₂ nanoparticles on the implant surface. In the green energy domain, the microwave device can be used to manufacture TiO₂ electrodes covered with noble metals [32] aiming to improve the photocatalysis system's efficiency for green hydrogen production.

## 4. Materials and Methods

The evolution of technology has allowed for the development of microwave emission sources (magnetron tubes) for commercial applications. In the scientific field, different microwave plasma devices have been developed [33]. In general, a microwave plasma system is based on a few basic components: a microwave source, a power supply, and a resonant cavity or a waveguide. A new microwave plasma generator built with commercial components was developed by our group to create a plasma and synthesize titanium oxide films and nanoparticles. It is known that when a metallic object is introduced in a microwave oven, electric sparks are generated [34]. To create a plasma following the interaction between microwaves and a metallic wire the multimode waveguide of a microwave oven was replaced with a single-mode waveguide (TM₀₁—transverse magnetic mode). The single-mode waveguide focuses the microwaves on a single point, which is the node of the cavity, where a high power density can be achieved.

The geometrical dimensions of the waveguide were calculated from Equation (1) [35]:

$$ (f_r)_{\text{mnl}}^{\text{TM}} = \left( \frac{1}{2\pi\sqrt{\mu \cdot \epsilon}} \right) = \sqrt{\left( \frac{p_{01}}{a} \right)^2 + \left( \frac{l\pi}{h} \right)^2} \quad (1) $$

where f_r—the resonance frequency of the waveguide; a—radius of the waveguide, h—length of the waveguide; l—longitudinal mode of the cavity; μ—permeability of the medium within the cavity (H/m); ε—permittivity of the medium within the cavity (F/m); P₀₁—first zero of the Bessel function (equal to ~2.405).

The indices mnl of the TM propagation mode refer to the number of half-wavelength variations in the radial, axial, and longitudinal directions. From Equation (1), the waveguide
has the following dimensions: 10.5 cm diameter, and 11 cm length. If a metallic wire, which is electrically isolated is placed with its tip in the focal point of the cavity, it will be irradiated by a high electric field when the power is applied. In atmospheric air, the high electric field generated at the tip of the metallic wire ionizes the gas atoms, and a plasma is created. The design of the new device is sketched in Figure 15.

<figure><img src="image_16.png" /><figcaption>**Figure 15.** Design of the microwave plasma generator. 1—pressure chamber, 2—magnetron, 3—magnetron antenna, 4—TM waveguide, 5—metallic wire, 6—metallic vapors deposition substrate, 7—NIR-VIS-UV Spectrometer, 8—ceramic support, 9—plasma.</figcaption></figure>

A commercial microwave oven is usually powered at 220 V, 50 Hz. The magnetron generates microwaves with frequency = 2.45 GHz in pulsed mode (20 ms pulses or 50 Hz). To control the microwave power emission of the magnetron an electronic controller was developed. To analyze the behavior of the titanium wires when these were exposed to microwaves we used wires with a length of 5 cm from a roll of 99.98% purity titanium wire with 1 mm diameter. Table 3 displays the chemical composition of the Ti wire before exposure to microwaves and Figure 16 displays the EDS spectrum acquired from the Ti wire.

<table><caption>**Table 3.** The chemical composition of the Ti wire before exposure to microwaves.</caption><thead><tr><td>Element</td><td>Weight %</td><td>Atomic %</td></tr></thead><tbody><tr><td>O K</td><td>4.22</td><td>11.65</td></tr><tr><td>Ti K</td><td>95.78</td><td>88.35</td></tr></tbody></table>

After positioning the titanium wire with one end in the focal point of the waveguide cavity, the power source of the magnetron was turned on, and then the power of the microwaves was increased to 800 W. After the plasma initiation process for the first Ti wire the microwaves power was set at 500 W and for the second Ti wire the microwaves power was set at 800 W. Following the interaction of the microwaves and the titanium wire, a plasma was generated.

The plasma generation process was set to 10 s for each experiment. In Figure 17a,b images of the plasma generated at 500 W and 800 W microwave power are displayed.
<figure><img src="image_17.png" /><figcaption>**Figure 16.** EDS spectrum from the Ti wire before exposure to microwaves.</figcaption></figure>

<figure><img src="image_18.png" /><figcaption>**Figure 17.** The microwaves discharge at 500 W RF (a) and 800 W RF (b) in air at atmospheric pressure: 1—waveguide, 2—the place where the silicon substrate was inserted, 3—magnetron antenna, 4—plasma, 5—ceramic support.</figcaption></figure>

**5. Conclusions**

Using a direct interaction between microwaves and an electric isolated Ti wire in the air at normal atmospheric pressure a plasma was generated. The plasma volume increases with increasing microwave power. The LTE conditions were fulfilled for plasmas generated at 500 W and 800 W microwave power. During plasma generation, Ti oxide layers and nanoparticles were synthesized. The vaporization time of titanium wire and the nanoparticles deposition mechanism depends on the microwave power from the waveguide. During the 10 s interaction time of the Ti wire with 800 W power of the microwave, a 5 mm length of the Ti wire was completely converted to TiOₓ nanoparticles.

The SEM and XRD analyses highlight that during microwave discharge at 500 W and 800 W microwave powers TiOₓ nanoparticles with the same dimension were generated.

The EDS analysis performed on the two samples (silicon substrate deposited with TiOₓ at 800 W microwave power and the growth of the TiOₓ layer on the Ti wire at 500 W microwave power) showed that the microwave power plays an important role in quantitative conversion from Ti wire in TiOₓ.
The water vapor or other impurities contained in the atmospheric air do not affect the purity of the TiOₓ nanoparticles generated during the interaction process. The TEM analysis indicates that most of the nanoparticles are either amorphous or nanocrystalline.

**Author Contributions:** Conceptualization, M.M. and G.M.; methodology, M.M., G.M, V.C., P.P. and A.P.; formal analysis, S.I.Z., G.C., C.I., P.P. and A.P.; investigation, M.M., G.M., S.I.Z., P.P., N.M., A.P., B.S.V. and C.D.C.; resources, S.I.Z., G.C, C.I., A.P., B.S.V. and C.D.C.; writing—original draft preparation, M.M., G.M. and V.C.; writing—review and editing, M.M., G.M. and V.C.; visualization, G.M. and N.M.; supervision, M.M. and V.C.; project administration, V.C.; funding acquisition, N.M., B.S.V. and C.D.C. All authors have read and agreed to the published version of the manuscript.

**Funding:** This work was supported by grants from the Ministry of Scientific Research, Innovation and Digitalization, projects codes: PN-IV-P2-2.2-MC-2024-0581-MC121, PN-IV-P2-2.2-MC-2024-0577-MC122, ELI-RO 19/2024, and Nucleu programme—LAPLAS VII, no. 30N/2023.

**Institutional Review Board Statement:** Not applicable.

**Informed Consent Statement:** Not applicable.

**Data Availability Statement:** Data is contained within the article.

**Acknowledgments:** The authors are grateful to the Romanian Government for providing access to the research infrastructure of the National Center for Micro and Nanomaterials through the National Program titled "Installations and Strategic Objectives of National Interest" and LaMP facilities at LP3-Marsille France.

**Conflicts of Interest:** The authors declare no conflicts of interest.

## References

1. Shi, H.; Magaye, R.; Castranova, V.; Zhao, J. Titanium dioxide nanoparticles: A review of current toxicological data. *Part. Fibre Toxicol.* **2013**, *10*, 15. [CrossRef] [PubMed]

2. Azizi-Lalabadi, M.; Ehsani, A.; Divband, B.; Alizadeh-Sani, M. Antimicrobial activity of Titanium dioxide and Zinc oxide nanoparticles supported in 4A zeolite and evaluation the morphological characteristic. *Sci. Rep.* **2019**, *9*, 17439. [CrossRef]

3. Assim, E.M. Optical constants of titanium monoxide TiO thin films. *J. Alloys Compd.* **2008**, *465*, 1-7. [CrossRef]

4. López-Huerta, F.; Cervantes, B.; González, O.; Hernández-Torres, J.; García-González, L.; Vega, R.; Herrera-May, A.L.; Soto, E. Biocompatibility and Surface Properties of TiO₂ Thin Films Deposited by DC Magnetron Sputtering. *Materials* **2014**, *7*, 4105-4117. [CrossRef] [PubMed]

5. Gázquez, M.J.; Bolívar, J.P.; Garcia-Tenorio, R.; Vaca, F. A Review of the Production Cycle of Titanium Dioxide Pigment. *Mater. Sci. Appl.* **2014**, *5*, 441-458. [CrossRef]

6. Blundell, R.; Butterworth, P.; Charlier, A.; Daurio, D.; Degenhardt, M.; Harris, D.; Hancock, B.; Johnston, M.; Kasina, R.; Kaye, J.; et al. The Role of Titanium Dioxide (E171) and the Requirements for Replacement Materials in Oral Solid Dosage Forms: An IQ Consortium Working Group Review. *J. Pharm. Sci.* **2022**, *111*, 2943-2954. [CrossRef]

7. Manurung, P.; Putri, Y.; Simanjuntak, W.; Low, I. Synthesis and characterisation of chemical bath deposited TiO₂ thin-films. *Ceram. Int.* **2013**, *39*, 255-259. [CrossRef]

8. Bessergenev, V.; Khmelinskii, I.; Pereira, R.; Krisuk, V.; Turgambaeva, A.; Igumenov, I. Preparation of TiO₂ films by CVD method and its electrical, structural and optical properties. *Vacuum* **2002**, *64*, 275-279. [CrossRef]

9. Fisher, P.; Maksimov, O.; Du, H.; Heydemann, V.D.; Skowronski, M.; Salvador, P.A. Growth, structure, and morphology of TiO₂ films deposited by molecular beam epitaxy in pure ozone ambients. *Microelectron. J.* **2006**, *37*, 1493-1497. [CrossRef]

10. Wang, Y.-H.; Rahman, K.H.; Wu, C.-C.; Chen, K.-C. A Review on the Pathways of the Improved Structural Characteristics and Photocatalytic Performance of Titanium Dioxide (TiO₂) Thin Films Fabricated by the Magnetron-Sputtering Technique. *Catalysts* **2020**, *10*, 598. [CrossRef]

11. György, E.; Socol, G.; Axente, E.; Mihailescu, I.; Ducu, C.; Ciuca, S. Anatase phase TiO₂ thin films obtained by pulsed laser deposition for gas sensing applications. *Appl. Surf. Sci.* **2005**, *247*, 429-433. [CrossRef]

12. Solomon, A. Synthesis, Modification, Applications and Challenges of Titanium Dioxide Nanoparticles. *Res. J. Nanosci. Eng.* **2019**, *3*, 10-22. [CrossRef]

13. Szczyglewska, P.; Feliczak-Guzik, A.; Nowak, I. Nanotechnology—General Aspects: A Chemical Reduction Approach to the Synthesis of Nanoparticles. *Molecules* **2023**, *28*, 4932. [CrossRef] [PubMed]
14. Chandoliya, R.; Sharma, S.; Sharma, V.; Joshi, R.; Sivanesan, I. Titanium Dioxide Nanoparticle: A Comprehensive Review on Synthesis, Applications and Toxicity. *Plants* **2024**, *13*, 2964. [CrossRef]

15. Uhm, H.S.; Hong, Y.C.; Shin, D.H. A microwave plasma torch and its applications. *Plasma Sources Sci. Technol.* **2006**, *15*, S26-S34. [CrossRef]

16. Whittaker, A.G.; Mingos, D.M.P. Arcing and other microwave characteristics of metal powders in liquid systems. *J. Chem. Soc. Dalton Trans.* **2000**, *9*, 1521-1526. [CrossRef]

17. Cheng, J.; Roy, R.; Agrawal, D. Experimental proof of major role of magnetic field losses in microwave heating of metal and metallic composites. *J. Mater. Sci. Lett.* **2001**, *20*, 1561-1563. [CrossRef]

18. Tanabe, E.; McEuen, A.; Trail, M.; Meddaugh, G.; Bandy, S. Field emission in microwave cavity. *Appl. Surf. Sci.* **1994**, *76-77*, 16-20. [CrossRef]

19. Mogildea, M.; Mogildea, G. Microwave field influence on the EMI 9656B photomultiplier tubes and NaI(Tl) crystal scintillator. *Optoelectron. Adv. Mater.-Rapid Commun.* **2018**, *12*, 713-718.

20. Popescu, S.; Jerby, E.; Meir, Y.; Barkay, Z.; Ashkenazi, D.; Mitchell, J.B.A.; Le Garrec, J.-L.; Narayanan, T. Plasma column and nano-powder generation from solid titanium by localized microwaves in air. *J. Appl. Phys.* **2015**, *118*, 023302. [CrossRef]

21. Feng, Y.; Wang, W.; Wang, Y.; Sun, J.; Zhang, C.; Shahzad, Q.; Mao, Y.; Zhao, X.; Song, Z. Experimental study of destruction of acetone in exhaust gas using microwave-induced metal discharge. *Sci. Total. Environ.* **2018**, *645*, 788-795. [CrossRef]

22. Mogildea, G.; Mogildea, M.; Popa, C.; Chiritoi, G. The Assessment of Carbon Dioxide Dissociation Using a Single-Mode Microwave Plasma Generator. *Molecules* **2020**, *25*, 1558. [CrossRef] [PubMed]

23. Mogildea, G.; Mogildea, M.; I Zgura, S.; Craciun, D.; Popa, C.; Prepelita, P.; Bazavan, M.C.; Craciun, V. The assessment of the atmospheric air breakdown voltage generated by the interaction between microwaves and metallic wires. *Phys. Scr.* **2023**, *98*, 045508. [CrossRef]

24. USB2000+ Data Sheet. Available online: https://ph208.edu.physics.uoc.gr/pdfs/OEM-Data-Sheet-USB2000-.pdf (accessed on 27 January 2025).

25. National Institute of Standards and Technology (NIST). Atomic Spectra Database. Available online: https://physics.nist.gov/ (accessed on 27 January 2025).

26. Bousquet, B.; Gardette, V.; Ros, V.M.; Gaudiuso, R.; Dell'Aglio, M.; De Giacomo, A. Plasma excitation temperature obtained with Boltzmann plot method: Significance, precision, trueness and accuracy. *Spectrochim. Acta Part B At. Spectrosc.* **2023**, *204*, 106686. [CrossRef]

27. Mogildea, M.; Mogildea, G.; Craciun, V.; Zgura, S.I. The Effects Induced by Microwave Field upon Tungsten Wires of Different Diameters. *Materials* **2021**, *14*, 1036. [CrossRef]

28. Ma, K.; Zhang, R.; Sun, J.; Liu, C. Oxidation Mechanism of Biomedical Titanium Alloy Surface and Experiment. *Int. J. Corros.* **2020**, *2020*, 1036. [CrossRef]

29. Barreca, F.; Acacia, N.; Barletta, E.; Spadaro, D.; Currò, G.; Neri, F. Titanium oxide nanoparticles prepared by laser ablation in water. *Radiat. Eff. Defects Solids* **2010**, *165*, 573-578. [CrossRef]

30. Ayorinde, T.; Sayes, C.M. An updated review of industrially relevant titanium dioxide and its environmental health effects. *J. Hazard. Mater. Lett.* **2023**, *4*, 100085. [CrossRef]

31. Cochran, D.L. A Comparison of Endosseous Dental Implant Surfaces. *J. Periodontol.* **1999**, *70*, 1523-1539. [CrossRef]

32. Kmetykó, Á.; Mogyorósi, K.; Gerse, V.; Kónya, Z.; Pusztai, P.; Dombi, A.; Hernádi, K. Photocatalytic H₂ Production Using Pt-TiO₂ in the Presence of Oxalic Acid: Influence of the Noble Metal Size and the Carrier Gas Flow Rate. *Materials* **2014**, *7*, 7022-7038. [CrossRef] [PubMed]

33. Khiabani, N.H.; Yaghmaee, M.S.; Sarani, A.; Shokri, B. Synthesis-Gas Production from CH₄-CO₂-Ar via Microwave Plasma Torch, *Adv. Stud. Theor. Phys.* **2012**, *6*, 1273-1287. Available online: https://www.m-hikari.com/astp/astp2012/astp25-28-2012/yaghmaeeASTP25-28-2012.pdf (accessed on 27 January 2025).

34. Bianchi, C.; Datta, A.; Dughiero, F. Mechanistic understanding of plasma arcing in microwave food processing. *Chem. Eng. Sci.* **2018**, *195*, 141-158. [CrossRef]

35. Souliez, F.; Chianese, S.; Dizac, G.; Micci, M. Low-power microwave arcjet testing—Plasma and plume diagnostics and performance evaluation. In Proceedings of the 35th Joint Propulsion Conference and Exhibit, Los Angeles, CA, USA, 20-24 June 1999. [CrossRef]

**Disclaimer/Publisher's Note:** The statements, opinions and data contained in all publications are solely those of the individual author(s) and contributor(s) and not of MDPI and/or the editor(s). MDPI and/or the editor(s) disclaim responsibility for any injury to people or property resulting from any ideas, methods, instructions or products referred to in the content.